Ternary rare-earth aluminium intermetallics RE10TAl3 (RE = Y, Ho, Tm, Lu; T = Fe, Co, Ni, Ru, Rh, Pd, Os, Ir, Pt) with an ordered anti-Co2Al5 structure.
Benndorf, Christopher; Eckert, Hellmut; Janka, Oliver; Dalton transactions (Cambridge, England : 2003) 46 (2017) 1083–1092; doi:10.1039/c6dt04314c

data_7041573
_publ_section_title
;
 Ternary rare-earth aluminium intermetallics RE10TAl3 (RE = Y, Ho, Tm, Lu;
 T = Fe, Co, Ni, Ru, Rh, Pd, Os, Ir, Pt) with an ordered anti-Co2Al5
 structure.
;
_journal_issue                   4
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1083
_journal_page_last               1092
_journal_paper_doi               10.1039/c6dt04314c
_journal_volume                  46
_journal_year                    2017
_chemical_formula_sum            'Al2.72 Lu10 Ni1.28'
_chemical_formula_weight         1898.2
_chemical_name_systematic        ' ?'
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   9.2985(4)
_cell_length_b                   9.2985(4)
_cell_length_c                   9.2702(4)
_cell_measurement_reflns_used    11714
_cell_measurement_temperature    293
_cell_measurement_theta_max      35.10
_cell_measurement_theta_min      2.53
_cell_volume                     694.14(5)
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'IPDS Stoe'
_diffrn_measurement_method       '??integration method??'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0768
_diffrn_reflns_av_unetI/netI     0.0142
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            16644
_diffrn_reflns_theta_full        34.94
_diffrn_reflns_theta_max         34.94
_diffrn_reflns_theta_min         2.53
_exptl_absorpt_coefficient_mu    72.168
_exptl_absorpt_correction_T_max  0.4994
_exptl_absorpt_correction_T_min  0.2603
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   Jana2006
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    9.0819
_exptl_crystal_description       block
_exptl_crystal_F_000             1561
_exptl_crystal_size_max          0.050
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.040
_refine_diff_density_max         2.83
_refine_diff_density_min         -3.47
_refine_ls_extinction_coef       2160(190)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.62
_refine_ls_goodness_of_fit_ref   1.52
_refine_ls_number_constraints    4
_refine_ls_number_parameters     21
_refine_ls_number_reflns         610
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0371
_refine_ls_R_factor_gt           0.0245
_refine_ls_shift/su_max          0.0016
_refine_ls_shift/su_mean         0.0002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0004I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0495
_refine_ls_wR_factor_ref         0.0516
_reflns_number_gt                495
_reflns_number_total             610
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            c6dt04314c1.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

'_exptl_absorpt_correction_type' value 'Gaussian' changed to
'gaussian' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7041572--7041573.cif.
;
_cod_original_sg_symbol_Hall     '-P 6c;-2c'
_cod_database_code               7041573